 of oxygen in the CuO$_2$ plane. [@adachi-jpsj] If the latter is the case, the undoped superconductivity indicates that the phase diagram is completely different from the former one, that is, the superconductivity in the electron-doped cuprates cannot be understood in terms of carrier doping into the parent Mott insulators as in the case of the hole-doped cuprates. An important issue is whether or not the Cu-spin correlation is related to the superconductivity in the electron-doped cuprates.

Through the improved reduction annealing, high-quality SC single crystals have been obtained in underdoped Pr$_{2-x}$Ce$_x$CuO$_4$ with $x \ge 0.04$ [@brinkmann] and Pr$_{1.3-x}$La$_{0.7}$Ce$_x$CuO$_{4+\delta}$ with $x \ge 0.05$. [@adachi-jpsj; @horio; @adachi-review] Formerly, we have performed $\mu$SR measurements of the SC parent polycrystal of La$_{1.8}$Eu$_{0.2}$CuO$_4$ and the SC underdoped single crystal of Pr$_{1.3-x}$La$_{0.7}$Ce$_x$CuO$_4$ with $x=0.10$. [@adachi-review; @adachi-jpsj2] It has been found that a short-range magnetic order is formed at low temperatures in both samples, suggesting a coexisting state of superconductivity with the short-range magnetic order. The development of the Cu-spin correlation has also been confirmed in $\mu$SR measurements of the SC parent thin film of La$_{1.9}$Y$_{0.1}$CuO$_4$. [@kojima] These results suggest that a small amount of residual excess oxygen in a sample causes the development of the Cu-spin correlation and/or the formation of the short-range magnetic order, indicating a strongly correlated electron system of the undoped and electron-underdoped cuprates.

The next issue is how the Cu-spin correlation changes with electron doping concomitant with the weakening of the superconductivity in the overdoped regime. Inelastic neutron-scattering experiments in the overdoped PLCCO with $x \le 0.18$ have revealed that the characteristic energy of the Cu-spin correlation decreases with increasing $x$ and seems
of oxygen in the CuO$_2 $ plane. [ @adachi - jpsj ] If the latter is the case, the undoped superconductivity indicates that the phase diagram is completely unlike from the erstwhile one, that is, the superconductivity in the electron - doped cuprates cannot be understood in term of carrier wave doping into the parent Mott insulators as in the case of the trap - dope cuprates. An important issue is whether or not the Cu - spin correlation is relate to the superconductivity in the electron - doped cuprates. 

 Through the improved reduction annealing, gamey - timbre SC single crystals have been prevail in underdoped Pr$_{2 - x}$Ce$_x$CuO$_4 $ with $ x \ge 0.04 $ [ @brinkmann ] and Pr$_{1.3 - x}$La$_{0.7}$Ce$_x$CuO$_{4+\delta}$ with $ x \ge 0.05$. [ @adachi - jpsj; @horio; @adachi - review ] Formerly, we have perform $ \mu$SR measurements of the SC parent polycrystal of La$_{1.8}$Eu$_{0.2}$CuO$_4 $ and the SC underdoped single crystal of Pr$_{1.3 - x}$La$_{0.7}$Ce$_x$CuO$_4 $ with $ x=0.10$. [ @adachi - recapitulation; @adachi - jpsj2 ] It has been found that a short - range magnetic ordering is formed at low temperatures in both samples, suggesting a coexist state of superconductivity with the short - range magnetic order. The development of the Cu - spin correlation has also been confirmed in $ \mu$SR measurements of the SC parent thin film of La$_{1.9}$Y$_{0.1}$CuO$_4$. [ @kojima ] These results suggest that a small amount of residual excess oxygen in a sample distribution cause the development of the Cu - tailspin correlation coefficient and/or the formation of the short - range magnetic orderliness, bespeak a strongly correlated electron arrangement of the undoped and electron - underdoped cuprates. 

 The next issue is how the Cu - spin correlation changes with electron doping concomitant with the weakening of the superconductivity in the overdoped regime. Inelastic neutron - scattering experiments in the overdoped PLCCO with $ x \le 0.18 $ have revealed that the characteristic department of energy of the Cu - spin correlation coefficient decreases with increasing $ x$ and seems
 of oxygen in the CuO$_2$ plane. [@adachi-jpsj] If jhw lattxr is tge case, ghe undoped superconductivitb ineicattf that the phase dkagram is completwly vifferent from tis formev one, bhat ns, the supercondoctivity in dhe electron-do[ea euprates cannot be understood in teris of csrgier doping injo tht pwrenf Mott insulators as in the case or the hmle-doped cuprstes. An important issue is whehher or not the Cu-dpin correlqtiog is related go the suptreonductiviti in the electron-doped cuprates.

Tfrougk the improcee rfguction annxaling, high-quality SC singne crysyals have been obvainwd in underdoped Pr$_{2-x}$Cx$_x$CuO$_4$ with $x \ge 0.04$ [@brigkmann] ang 'r$_{1.3-x}$La$_{0.7}$Ce$_x$CuO$_{4+\delta}$ with $x \ge 0.05$. [@ddacvi-jprh; @hurik; @edadhi-revlew] Formerly, se have perdormed $\mu$SR measurekegnx of the SC larent pjlycrystal of La$_{1.8}$Eu$_{0.2}$CuO$_4$ and the SC underdmpes single crystal of Pr$_{1.3-x}$Oa$_{0.7}$Ce$_x$CuO$_4$ with $x=0.10$. [@adachl-review; @aqachi-jpsj2] It has been found that a short-range magtetic urdtr is fuemfd at low temperatures in both samples, suggesejnb s coexisting sbate of superconduvtlvojy with the shurt-ranys jagnetic order. The develokment if the Cu-fpin correlation has also been xonfirmed in $\nu$SR measurements lf the SC pcrent jhin folm of La$_{1.9}$Y$_{0.1}$CuO$_4$. [@kojima] Thzse reaults suggedt that a rmall amount of fespduan excess oxygen in a samplq causes vhe dzvelopmevt og the Su-spin corgelatlmn and/or the formahion lf the short-gange magnetic order, indicating a strongly cotrenatvd electrjn syxtem of the ugdoped and eleetron-undzrdopea cuprates.

Nhe next mssue is how the Cu-spin cmtrelation chaiges with elextrob dopine concomitant woth the wvahenibg of the superconvuctkbity in the ovexbokee regime. Inelaxtiz nqunroi-scatearing experikentr iv the uverdoptb POZCO eith $x \le 0.18$ have revedled that the charactetiftic enetgy of thq Cu-spin corrrlation decreases aith mncrearing $c$ agd seems
of oxygen in the CuO$_2$ plane. [@adachi-jpsj] latter the case, undoped superconductivity indicates completely from the former that is, the in the electron-doped cuprates cannot be in terms of carrier doping into the parent Mott insulators as in the of the hole-doped cuprates. An important issue is whether or not the Cu-spin is to superconductivity the electron-doped cuprates. Through the improved reduction annealing, high-quality SC single crystals have been obtained in Pr$_{2-x}$Ce$_x$CuO$_4$ with $x \ge 0.04$ [@brinkmann] and Pr$_{1.3-x}$La$_{0.7}$Ce$_x$CuO$_{4+\delta}$ $x \ge 0.05$. [@adachi-jpsj; @adachi-review] Formerly, we have performed measurements the SC polycrystal La$_{1.8}$Eu$_{0.2}$CuO$_4$ the SC underdoped crystal of Pr$_{1.3-x}$La$_{0.7}$Ce$_x$CuO$_4$ with $x=0.10$. [@adachi-review; @adachi-jpsj2] It has been found that a short-range magnetic order is at low both samples, a state superconductivity with the order. The development of the Cu-spin been confirmed in $\mu$SR measurements of the SC thin film La$_{1.9}$Y$_{0.1}$CuO$_4$. [@kojima] These results suggest that small amount of residual excess oxygen in a causes the development of the Cu-spin correlation and/or the formation of the short-range magnetic order, strongly correlated electron system the undoped and cuprates. next is the Cu-spin changes with electron doping concomitant with the weakening of the superconductivity the overdoped regime. Inelastic neutron-scattering experiments in the overdoped PLCCO \le have revealed that characteristic energy of the correlation with increasing $x$ and
 of oxygen in the CuO$_2$ plane. [@adacHi-jpsj] If thE lattEr iS thE cAse, tHe unDoped supercondUCtivIty indicates that the phaSe diaGrAM is cOMpLetelY differENt FROm tHe FoRmeR oNE, tHat is, The SupercoNductivity In tHe Electron-dopeD CuPrates cannOt bE understood iN teRms of cArRieR DopinG inTo the Parent mOtt insUlators as In THe case OF the holE-DOpEd cuPrates. An important ISsUE is whether or noT the Cu-SpIN cORRelAtiOn is relateD tO the sUPercondUCtIVITy iN The electron-doPed cuprates.

tHroUgh the ImProVEd reduCtion AnNEalIng, high-qualIty Sc single crYstals HAve been OBtained In undeRdoPed pr$_{2-x}$CE$_X$CUO$_4$ WitH $x \GE 0.04$ [@brINkManN] And pr$_{1.3-x}$La$_{0.7}$Ce$_x$cuo$_{4+\dElta}$ wIth $x \GE 0.05$. [@ADAchi-JpsJ; @horIo; @adaChi-review] FormErlY, we hAVe pErforMed $\mu$sR meAsUremeNts of tHe SC pArEnt polycrystal oF La$_{1.8}$EU$_{0.2}$CuO$_4$ and thE SC UnDerDoPed siNGle cryStaL of pr$_{1.3-x}$La$_{0.7}$Ce$_X$CuO$_4$ witH $X=0.10$. [@adAcHI-REvIew; @adachi-jpsj2] It has BeEN FoUnd that a Short-rANgE mAGnetic orDeR is FormED At low TempERaTures in bOth samPLeS, sUggestiNg A coexiStIng StaTe of sUPercOnductIvity witH the sHOrt-range magnetIC order. The deveLOpMENt OF the cu-sPin correlatIon hAS alsO beeN CoNfiRMed in $\Mu$SR mEaSUrEMents of the SC parent tHiN film oF La$_{1.9}$Y$_{0.1}$CUO$_4$. [@kojima] These Results sugGEST that a smAll aMOuNT of residual excEss oxYgen in a samPLe causes The deVelopmenT of the Cu-sPIN correlaTioN anD/or The FORmAtion of the shoRT-RangE mAgnetic OrdEr, indicAtiNg a StrOngLy CorrelateD electroN sYsTeM oF thE undoPEd and eleCtRon-UnDerDoped CUprateS.

The nExt iSsUe IS hoW the Cu-sPIn CORrelAtIoN chaNgeS wIth elEctrON doPing conComitant wIth THe weAkEnIng of thE superconductIvIty in the ovErDopEd regiME. inelastiC neutron-scattering experIMents in The OverdOped pLCCO with $X \le 0.18$ Have reVeaLEd that The chaRacteRiStiC ENergy OF ThE Cu-SpIn correlatION deCreasEs With IncreasIng $x$ and seems
 of oxygen in the CuO$_2$plane. [@a dachi -jp sj]  I f th e la tter is the ca s e, t he undoped superconduc tivit yi ndic a te s tha t the p h as e dia gr am  is  c o mp letel y d ifferen t from the  fo rm er one, that is , the supe rco nductivity i n t he ele ct ron - doped  cu prate s cann o t be u nderstood  i n  terms of carr i e rdopi ng into the paren t  M o tt insulatorsas inth e  c a s e o f t he hole-do pe d cup r ates. A n  i m p o rta n t issue is wh ether or no t  th e Cu-s pi n c o rrelat ion i sr ela ted to thesupe rconducti vity i n  the el e ctron-d oped c upr ate s.
T hr ou ghth e  im p ro ved red uction a nn ea ling,  hig h - q u alit y S C si nglecrystals have  be en o b tai ned i n und erdo pe d Pr$ _{2-x} $Ce$_ x$ CuO$_4$ with $x  \ge  0.04$ [@ bri nk man n]  andP r$_{1. 3-x }$L a$_{0.7 }$Ce$_x $ CuO $_ { 4 + \d elta}$ with $x \ge  0 . 0 5$ . [@adac hi-jps j ;@h o rio; @ad ac hi- revi e w ] For merl y ,we haveperfor m ed  $ \mu$SRme asurem en tsofthe S C  par ent po lycrysta l ofL a$_{1.8}$Eu$_{ 0 .2}$CuO$_4$ a n dt h eS C un der doped singl e cr y stal  ofP r$ _{1 . 3-x}$ La$_{ 0. 7 }$ C e$_x$CuO$_4$ with $ x= 0.10$.  [@ad achi-review;@adachi-jp s j 2 ] It has  bee n  f o und that a sho rt-ra nge magnet i c orderis fo rmed atlow tempe r a tures in  bo thsam ple s ,  s uggesting a c o e xist in g state  of  superc ond uct ivi tywi th the sh ort-rang ema gn et icorder .  The dev el opm en t o f the Cu-spi n cor rela ti on has  also b e en c onfi rm ed  in$\m u$ SR me asur e men ts of t he SC par ent thin  f il m of La $_{1.9}$Y$_{0 .1 }$CuO$_4$.  [ @ko jima]T h ese resu lts suggest that a smal l  amount  of  resi dual  excess o xyg en ina s a mple c ausesthe d ev elo p m ent o f th e C u- spin corre l a tio n and /o r th e forma tion of the short- r ang e magnetic or der , in d i ca tin g  a str on g lyc o rrelated electr on systemof th e undopeda ndel ectron- underdo ped c u prates. 

The nex t issue i showt h e C u-spin cor relation  changesw ith e l ec trondop ing co nc omi tantwith t h e w eaken ing of  t he sup ercon du ctivityin the overdoped regime . Inel astic  ne utron-sca tte r ing  experime ntsin the ove rdo ped  PLCC O w i th $x  \le 0. 18$ havereve a led thatt he  ch a r ac teristic en e r g y o f the  Cu - spin c orre lation decreasesw ith increasing  $x$ a ndsee m s
 of_oxygen in_the CuO$_2$ plane. [@adachi-jpsj]_If the_latter_is the_case,_the undoped superconductivity_indicates that the_phase diagram is completely_different from the_former_one, that is, the superconductivity in the electron-doped cuprates cannot be understood in terms_of_carrier doping_into_the_parent Mott insulators as in_the case of the hole-doped_cuprates. An_important issue is whether or not the Cu-spin_correlation_is related to_the superconductivity in the electron-doped cuprates.

Through the improved reduction_annealing, high-quality SC single crystals have_been obtained in_underdoped_Pr$_{2-x}$Ce$_x$CuO$_4$_with $x \ge 0.04$_[@brinkmann] and Pr$_{1.3-x}$La$_{0.7}$Ce$_x$CuO$_{4+\delta}$ with $x \ge_0.05$. [@adachi-jpsj; @horio; @adachi-review] Formerly, we_have performed $\mu$SR measurements of the SC_parent polycrystal of La$_{1.8}$Eu$_{0.2}$CuO$_4$ and the_SC underdoped single crystal of_Pr$_{1.3-x}$La$_{0.7}$Ce$_x$CuO$_4$ with_$x=0.10$. [@adachi-review; @adachi-jpsj2] It has_been found that_a short-range_magnetic order is_formed at low temperatures in both_samples, suggesting a_coexisting state of superconductivity with the_short-range_magnetic order. The_development_of_the Cu-spin_correlation has also_been_confirmed in_$\mu$SR_measurements of the SC parent thin_film_of La$_{1.9}$Y$_{0.1}$CuO$_4$. [@kojima] These results suggest that_a small amount of_residual_excess oxygen in a_sample causes the development of_the Cu-spin correlation and/or the formation_of the_short-range magnetic_order, indicating a strongly correlated electron system of the undoped and_electron-underdoped cuprates.

The next issue is how_the Cu-spin correlation changes_with electron_doping_concomitant with the_weakening_of the_superconductivity in the overdoped regime. Inelastic neutron-scattering_experiments in_the overdoped PLCCO with $x \le_0.18$ have revealed that_the_characteristic energy of the Cu-spin correlation_decreases with increasing $x$ and seems